| ||Format||Pages||Price|| |
|21||$72.00||  ADD TO CART|
|Hardcopy (shipping and handling)||21||$72.00||  ADD TO CART|
This specification covers the requirements and test procedures for materials, dimensions, hydrostatic burst strength, chemical resistance, peeling strength, adhesion strength, and tensile strength properties for cured-in-place (CIP) pipe liners installed into existing metallic gas pipes for rehabilitation purposes. These cured-in-place pipe liners are intended for use in pipelines that transport natural gas, petroleum fuels (propane-air and propanebutane vapor mixtures), and manufactured and mixed gases, where resistance to gas permeation, ground movement, internal corrosion, leaking joints, pinholes, and chemical attack are required. The materials, which shall be considered separately for testing, consist of the flexible tubing, jacket, elastomer skin, and adhesive system.
This abstract is a brief summary of the referenced standard. It is informational only and not an official part of the standard; the full text of the standard itself must be referred to for its use and application. ASTM does not give any warranty express or implied or make any representation that the contents of this abstract are accurate, complete or up to date.
1.1 This specification covers requirements and method of testing for materials, dimensions, hydrostatic burst strength, chemical resistance, adhesion strength and tensile strength properties for cured-in-place (CIP) pipe liners installed into existing metallic gas pipes, 3/4 to 48 in. nominal pipe size, for renewal purposes. The maximum allowable operating pressure (MAOP) of such renewed gas pipe shall not exceed a pressure of 300 psig (2060 kPa). The cured-in-place pipe liners covered by this specification are intended for use in pipelines transporting natural gas, petroleum fuels (propane-air and propane-butane vapor mixtures), and manufactured and mixed gases, where resistance to gas permeation, ground movement, internal corrosion, leaking joints, pinholes, and chemical attack are required.
1.2 The medium pressure (up to 100 psig) cured-in-place pipe liners (Section A) covered by this specification are intended for use in existing structurally sound or partially deteriorated metallic gas pipe as defined in . The high pressure (over 100 psig up to 300 psig) cured-in-place pipe liners (Section B) covered by this specification are intended for use only in existing structurally sound steel gas pipe as defined in . CIP liners are installed with limited excavation using an inversion method (air or water) and are considered to be a trenchless pipeline rehabilitation technology. The inverted liner is bonded to the inside wall of the host pipe using a compatible adhesive (usually an adhesive or polyurethane) in order to prevent gas migration between the host pipe wall and the CIP liner and, also, to keep the liner from collapsing under its own weight.
1.2.1 Continued growth of external corrosion, if undetected and unmitigated, could result in loss of the host pipe structural integrity to such an extent that the liner becomes the sole pressure bearing element in the rehabilitated pipeline structure. The CIP liner is not intended to be a stand-alone pipe and relies on the structural strength of the host pipe. The operator must maintain the structural integrity of the host pipe so that the liner does not become free standing.
1.3 MPL CIP liners (Section A) can be installed in partially deteriorated pipe as defined in . Even for low pressure gas distribution systems, which typically operate at less than 1 psig, MPL CIP liners are not intended for use as a stand-alone gas carrier pipe but rely on the structural integrity of the host pipe. Therefore, the safe use of cured-in-place pipe lining technology for the rehabilitation of existing cast iron, steel, or other metallic gas piping systems, operating at pressures up to 100 psig, is contingent on a technical assessment of the projected operating condition of the pipe for the expected 30 to 50 year life of the CIP liner. Cured-in-place pipe liners are intended to repair/rehabilitate structurally sound pipelines having relatively small, localized defects such as localized corrosion, welds that are weaker than required for service, or loose joints (cast iron pipe), where leaks might occur.
1.3.1 HPL CIP liners (Section B) are intended for use only in existing structurally sound steel gas pipe as defined in . HPL CIP liners are not intended for use as a stand-alone gas carrier pipe but rely on the structural integrity of the host pipe. Therefore, the safe use of cured-in-place pipe lining technology for the rehabilitation of existing steel gas piping systems, operating at pressures up to 300 psig, is contingent on a technical assessment of the projected operating condition of the pipe for the expected 30 to 50 year life of the CIP liner.
1.4 The values stated in inch-pound units are to be regarded as standard. No other units of measurement are included in this standard.
1.5 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use.
1.6 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
D123 Terminology Relating to Textiles
D543 Practices for Evaluating the Resistance of Plastics to Chemical Reagents
D763 Specification for Raw and Burnt Umber Pigments
D883 Terminology Relating to Plastics
D1598 Test Method for Time-to-Failure of Plastic Pipe Under Constant Internal Pressure
D1600 Terminology for Abbreviated Terms Relating to Plastics
D1763 Specification for Epoxy Resins
D2240 Test Method for Rubber PropertyDurometer Hardness
D2837 Test Method for Obtaining Hydrostatic Design Basis for Thermoplastic Pipe Materials or Pressure Design Basis for Thermoplastic Pipe Products
D3167 Test Method for Floating Roller Peel Resistance of Adhesives
D3892 Practice for Packaging/Packing of Plastics
D4814 Specification for Automotive Spark-Ignition Engine Fuel
D4848 Terminology Related to Force, Deformation and Related Properties of Textiles
D4850 Terminology Relating to Fabrics and Fabric Test Methods
F412 Terminology Relating to Plastic Piping Systems
ICS Number Code 23.040.15 (Non-ferrous metal pipes)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM F2207-06(2019), Standard Specification for Cured-in-Place Pipe Lining System for Rehabilitation of Metallic Gas Pipe, ASTM International, West Conshohocken, PA, 2019, www.astm.orgBack to Top